Magnon excitations and quantum critical behavior of the ferromagnet URuGe
Abstract
We present an extensive study of the ferromagnetic heavy fermion compound URuGe. Measurements of electrical resistivity, specific heat and magnetic properties show that URuGe orders ferromagnetically at ambient pressure with a Curie temperature K. The low temperature magnetic behavior of this soft ferromagnet is dominated by the excitation of gapless spinwave modes. Our results on the transport properties of URuGe under pressures up to GPa suggest that URuGe has a putative ferromagnetic quantum critical point (QCP) at GPa. In the ordered phase, ferromagnetic magnons scatter the conduction electrons and give rise to a well defined power law temperature dependence in the resistivity. The coefficient of this term is related to the spinwave stiffness and measurements of the very low temperature resistivity allow to accompany the behavior of this quantity as the the ferromagnetic QCP is approached. We find that the spinwave stiffness decreases with increasing pressure implying that the transition to the nonmagnetic Fermi liquid state is driven by the softening of the magnons. The observed quantum critical behavior of the magnetic stiffness is consistent with the influence of disorder in our system. At quantum criticality ( GPa), the resistivity shows the behavior expected for an itinerant metallic system near a ferromagnetic QCP.
I Introduction
The problems related to strongly correlated electronic systems are of great current interest due to the novel states of matter that can arise in these systems (2). These include their exotic magnetic properties, superconducting behavior and their phase diagrams, which exhibit quantum critical points (QCPs) (3). QCPs are experimentally explored by doping, applied pressure or magnetic field . In the case of actinide materials, the interesting properties arise from partially filled orbitals that strongly hybridize with the conduction electrons. This, together with the strong correlations among the states give rise to a variety of ground states.
The ternary compound URuGe is a system with interesting magnetic properties. It has a centered body (bcc) crystalline structure of the type UReSi (4). The lattice parameter is Å, and the interatomic space between the Uranium is Å(5), much larger than the Hill boundary for Uranium: Å, which sets conditions for a magnetic ground state (6). The compound URuGe has the properties of a heavy fermion system, with a Kondo resistivity and a large linear term in the low temperature specific heat (5). It orders ferromagnetically at low temperatures due to the small volume of its unit cell, which favors the RKKY interaction (5); (7); (8). Its ferromagnetism is characterized as itinerant, although Mentink et al. (5) propose localized ferromagnetism, contrary to other works in the literature (9); (10); (11). Under applied pressure, transport measurements show no evidence of discontinuous behavior as the ferromagnetic phase is suppressed and a nonmagnetic Fermi liquid state is attained (10).
In this work, we present an extensive study of the magnetic, thermodynamic and transport properties of URuGe (11) under applied magnetic field and of the latter under high applied pressures. We show that this system below its ambient pressure ferromagnetic transition at K has its low temperature properties dominated by the presence of low energy spinwave excitations. In systems with strong magnetocrystalline anisotropy as compounds containing states, these modes are generally quenched at low temperatures by the existence of a gap in the spinwave spectrum due to this anisotropy. However, URuGe is a unique system among the actinide materials with a negligible magnetocrystalline anisotropy (11). This allows for the excitation of magnons at very low temperatures and these modes end up having a prominent role on its low temperature physical properties, as we show here. In particular magnons scatter the conduction electrons and have a definite importance in the electrical resistivity of ferromagnetic metals. As we apply pressure on URuGe and measure its resistivity, we have a rare opportunity to observe the evolution of the spinwave stiffness of a ferromagnetic system as it approaches the QCP. Our transport measurements show a clear softening of the magnon modes as URuGe is driven to the putative ferromagnetic QCP (FQCP) with increasing pressure. In the present study, we obtain the quantum critical behavior of the stiffness of these excitations.
Ii Experimental
The sample was prepared by arc melting of its high purity metallic constituents in the ratio U:Ru:Ge = 1:2:2, under argon atmosphere, without further heat treatment, as to form the compound URuGe. However, the Xray diffractogram at room temperature showed a composition of URuGe, with additional spurious phases, as discussed in detail below. The Xray powder diffraction (XRD) at room temperature was performed using the Bruker AXS D8 Advance II diffractometer, with LynxEye detector, Cu source with K radiation.
The diffraction pattern was collected in a BraggBrentano configuration covering the angular range of to degrees, each step incremented by degree. The XRD data were refined using the Rietveld method (17), implemented in the program FullProf (18), available at the Institut LaueLangevin (ILL) website (19). The profile function used to adjust the shape of the diffraction peaks was the pseudoVoigt function.
Pressuredependent resistivity measurements were carried out in a temperature range from 0.1 K to 10 K in a noncommercial Adiabatic Demagnetization Refrigerator (ADR). A standard 2.5 GPa piston cylinder type of cell was used, with a mixture of fluorinert FC70FC77 as pressure medium, pure lead as pressure sensor at low temperatures and manganin as a manometer for loading the cell at ambient temperature. We further performed measurements of electrical resistivity under magnetic fields up to 9 T and respective magnetoresistance measurements in the temperature range from 1.8 K to 30 K in a commercial PPMS Dynacool from Quantum Design, at ambient pressure.
The specific heat measurements as a function of temperature were also performed in the PPMS DynaCool under different magnetic field values ranging from 0 to 7 T, in the temperature interval from 2 K to 15 K.
The magnetic characterization involved the application of external magnetic fields in DC and AC modes. The DC magnetization measurements were in field cooling (FC) mode in a field of 10 mT. For the AC susceptibility measurement, the parameters used were mT and mT at 3 kHz. Both type of measurements were performed from 2 K to 300 K in PPMS DynaCool, Quantum Design.
Iii Sample analysis
The XRD showed that the sample produced has a main phase of cubic crystalline structure of URuGe and secondary phases. After a detailed analysis of the diffraction pattern and identification of all peaks of minor intensities, it was found that the secondary phases could probably be RuGe and U. The Rietveld refinement of the Xray diffractogram was performed using first the URuGe main compound phase. In the sequence, the CIF data of the other phases were added in the base of the program; after adjustment, the presence of RuGe and U compounds was confirmed as secondary phases in the sample. The CIF data were obtained from the Inorganic Crystal Structure Database (ICSD).
Fig. 1 shows the refinement of the XRD, where the black circles are the experimentally observed data, while the solid red line is the standard calculated by the refinement. The allowed Bragg positions are represented in vertical green bars, where each level corresponds to the peaks of the Bragg planes of each of the phases found. The planes (hkl) shown in the figure correspond to the peaks of the diffractogram of the predominant phase URuGe, which appears in the amount of 78.08%. The parameters of the crystalline lattice and the amounts of each of the phases found as results of the refinement, as well as their quality R factors, are described in Table 1. The crystallographic datasheet ICSD 192067 (9) was used for the refinement of the phase URuGe. In Table 1, it is seen that the lattice parameters of all phases are in agreement with the literature (5); (7); (21); (22). The interatomic distance of the Uranium of the major phase URuGe is d = 5.866 Å, also agreeing with the literature (5); (7).
While Uranium in its allotropic forms has a higher resistivity than copper (25), it has a weak paramagnetic behavior, exhibiting paramagnetism almost independent of temperature (26); (27); the second spurious phase of the sample, RuGe, is semiconductor and strongly diamagnetic, exhibiting a paramagnetic contribution above 900 K due to the structural transition (28), from orthorhombic (centersymmetric) to tetragonal (nonsymmetrical) (29). Thus, in this work, we state that the low temperature magnetic, thermodynamic and transport properties of our sample are due to the main phase URuGe with negligible contribution from the secondary phases.
Phase  URuGe  RuGe  U 

Composition  78.06%  20.78 %  1.16% 
Crystalline structure  cubic  orthorhombic  cubic 
Space group  Im  Pbcn  Imm 
Datasheet CIFICSD  192067  85205  44392 
Lattice parameter  
a (Å)  8.295813  11.436  3.504737 
b (Å)    9.238   
c (Å)    5.716   
Iv Magnetic properties and evidence for spinwaves
The inverse of the magnetic ACsusceptibility of our sample as a function of temperature is shown in Fig. 2 from 2 K to 18 K. The data shows a peak at K that we identify as the Curie temperature, below which URuGe becomes ferromagnetic. This coincides with the found in Ref. (5) ( K), but is smaller than those found in Refs. (7); (10) that range in the interval between K. Above the susceptibility follows a CurieWeiss law from which we extract an effective magnetic moment of per Uranium atom (30). This is large compared to the value obtained from the saturation magnetization in large magnetic fields ( per Uranium atom) (5); (11), but smaller than the value of 2.54 extracted from the CurieWeiss behavior of the susceptibility at high temperatures (300 K T 500 K) (7). It is interesting that the CurieWeiss temperature indicated by an arrow in Fig. 2 is very close to the ferromagnetic critical temperature obtained from the peak in . This meanfield behavior is consistent with the rather large Uranium moment in a cubic structure and indicates that ferromagnetic fluctuations are important only close to .
In ferromagnetic systems, metallic or insulators, below the low temperature magnetic elementary excitations are long wavelength spinwaves with dispersion relation . The gap may be due to the magnetocrystalline anisotropy, dipolar interactions or to the Zeeman energy if an external magnetic field is applied in the material. The quantity is the spinwave stiffness of the magnetic system. For a soft ferromagnet with negligible anisotropy, in zero field and in the temperature range of our experiments, the gap in general can be neglected and the spectrum is purely quadratic in the wavevector . Notice that in this case, the mode is the Goldstone mode of the rotational invariant system (3).
Fig. 3 shows the low temperature behavior of , the molar specific heat divided by temperature, of URuGe. We took into account that only 78% of the total molecular weight is due to the main phase. The data is plotted in such a way to put in evidence a contribution proportional to associated with gapless ferromagnetic magnons with a quadratic dispersion. There is also a large linear temperature dependent term that is due to the heavy quasiparticles of the metallic URuGe compound. A phonon contribution to the specific heat becomes apparent in a plot of versus , where a linear behavior is observed in the temperature interval from 15 K to 30 K. The Debye temperature obtained from the inclination of this line is K (5). The data shows that this phonon contribution can be safely neglected in the temperature region below . The coefficient of the linear temperature dependent term of the specific heat obtained from the fit in Fig. 3 with is mJ/mol U K, similar to that given in the literature for this material (5); (10); (11). The coefficient of the spinwave contribution obtained from this fit is J/mol K. In spinwave theory, for a cubic ferromagnetic system with gapless magnon excitations, the expression for the contribution of these modes to the low temperature specific heat per unit volume is calculated as (12),
(1) 
This expression allows to obtain the spinwave stiffness from the coefficient of the term of the specific heat in the experimental data as shown in Fig. 3. Notice that with given by Eq. 1 and the molar volume. We get, using the value of above, meV Å. The error here is mainly due to uncertainty in the volume of the sample.
Fig. 4 shows the normalized low temperature magnetization of URuGe as a function of . The linear behaviour of the magnetization in this plot implies that at low temperatures it decreases according to a Bloch’s law. This is a clear signature that this decrease is due to the thermal excitation of ferromagnetic magnons (12). Bloch’s law yields,
(2) 
at low temperatures (12). The coefficient is related to the spinwave stiffness by (12),
(3) 
Using the experimental value of obtained from Fig. 4 in Eq. 3, we find meV Å, where the error comes from the uncertainty on the volume of the sample. In Eq. 2, M(0)= 6.1 x 10 emu/m
The values for the spinwave stiffness obtained above from the low temperature specific heat and magnetization measurements, meV Å and meV Å respectively, are consistent and of the expected order of magnitude for a soft metallic ferromagnet with a Curie temperature of K. For example, in ferromagnetic Ni with K (12) the experimentally obtained spinwave stiffness ranges from meV Å to meV Å (13), if extracted from Bloch’s law or measured directly by neutron scattering, respectively. These results strongly support the idea that ferromagnetic magnons play an important role in the thermodynamic properties of the cubic ferromagnetic URuGe below its Curie temperature.
V Transport properties
In ferromagnetic metals, the scattering of conduction electrons by ferromagnetic spinwaves gives rise to a temperature dependent contribution to the electrical resistivity of these materials (14). This contribution has indeed been found in a previous study of URuGe (10), but it has been attributed to electronelectron scattering as in strongly correlated paramagnetic metals. However, in a longrange ordered ferromagnetic metal, with polarized bands, and gapless spinwave modes, the main scattering is due to these elementary excitations. In fact, this is the main form electronelectron scattering assumes in an itinerant ferromagnetic metal. Here, we give evidence that in ferromagnetic URuGe substantial part of the term in its resistivity is due to electronmagnon scattering. This contribution to the resistivity is given by (14),
(4) 
where is a constant with units of resistivity, and , the Fermi wavevector and Fermi energy of the electrons, respectively. The quantity where is the maximum wavevector for which the quadratic spinwave dispersion relation, , holds. The spinwave stiffness appears in the denominator of this equation, such that, the softer the magnon modes the larger is this contribution to the resistivity. At a FQCP, where the spinwave stiffness vanishes, the resistivity of the metal is given by(14),
(5) 
In the next section, we will present results for the electric resistivity of our sample as a function of temperature for different applied pressures and magnetic fields. As pressure increases, the ferromagnetic Curie temperature vanishes smoothly at a FQCP at a critical pressure, GPa. The resistivity curves we obtain present no hysteresis for any pressure. We find no evidence of a behavior that could indicate a first order transition as the Curie temperature of the sample is reduced and made to vanish. As we accompany the variation of the coefficient of term with increasing pressure, we observe a smooth increase of this coefficient that we attribute entirely, according to Eq. 4, to a decrease of the spinwave stiffness as the FQCP is approached. At the critical pressure the resistivity follows a behavior in agreement with Eq. 5.
v.1 Pressure experiments
Fig. 5 shows the low temperature behavior of the electrical resistivity of URuGe as a function of pressure. All pressure experiments were carried out in zero external magnetic field.
The electrical resistivity behaves smoothly, with no detectable hysteresis for all pressures of the experiments. At very low temperatures, it presents a dependence, both above and below the critical pressure GPa and is well described by, . The exception is for pressures very close to where , as shown in Fig. 6. This is the expected power law behavior for a ferromagnetic metallic system close to a FQCP (see Eq. 5).
In Fig. 7, we show physical parameters obtained from the resistivity data as a function of pressure.

In principle, the observation of a clear cutbend (or kink) in the dependence of electrical resistivity is an indication of an onset of magnetic ordering. The precise determination of is obtained from the second derivative of the smoothed electrical resistivity data (15). In the upper panel of Fig. 7, we have plotted the obtained in this way and draw through these points a curve from a fit using the expected power law behavior for an itinerant FQCP, , where the shift exponent (3) , since the dynamic exponent is in this case (3). The curve gives a reasonable description of the pressure dependent Curie temperatures.

The next panel shows the pressure dependence of the residual resistivity. This is nearly constant in the ferromagnetic phase, with a small drop close to the critical pressure.

The last two panels refer to the pressure dependence of the coefficient of the term of the resistivity. They rise on both sides of the phase diagram as the critical pressure is approached from below and above in a nonsymmetric fashion. In the paramagnetic phase, above , this term is due to scattering by paramagnons and its coefficient is proportional to the square of the inverse of the coherence temperature (16), , with for a three dimensional itinerant ferromagnetic system (16). As can be seen in the last two panels, we do not have enough data for close to the critical pressure to be able to determine its power law dependence with the distance from criticality. Sufficiently far from , depends linearly on this distance, which suggests local quantum critical behavior (3).

For pressures below , in the ferromagnetic phase, according to Eq. 4 the coefficient of the term in the resistivity is related to spinwave stiffness , . In itinerant 3d ferromagnets, the coupling of the order parameter to particlehole excitations give rise to a nonanalytic behavior of the spinwave stiffness as a function of the magnetization (39). For a disordered quantum itinerant 3d ferromagnet,
(6) while for the clean system,
(7) where and are positive constants (39). In a 3d quantum metallic ferromagnet the magnetization vanishes close to the FQCP as with a meanfield exponent . In Fig. 8 we plot the pressure dependence of the quantity that mimics that of the spinwave stiffness for pressures approaching the FQCP. We compare the simple meanfield result with the results of Eqs. 6 and 7. The results for the clean and disordered ferromagnet are rather similar, but clearly they give a better description of the data than the simple meanfield.
Vi Effect of an external magnetic field
In this section, we study the effect of an applied magnetic field on the thermodynamic and transport properties of our sample at ambient pressure. In ferromagnets, a magnetic field is the conjugate of the order parameter and destroys the thermodynamic phase transition. This is different from the antiferromagnet where a uniform magnetic field just shifts the transition. The low temperature magnetic excitations of the ferromagnet in an external magnetic field are still magnons, but they become partially quenched by a Zeeman gap due to the coupling of the magnetic moments to the field.
This reduces the influence and contribution of spinwaves to the low temperature properties, i.e., for , where is the Zeeman gap.
In Fig. 9 we show the specific heat as a function of temperature in an applied field of 7 T. The low temperature specific heat is well fitted by the expression . The exponential term takes into account the quenching of the magnons by the Zeeman gap , expressed here in temperature scale. From this fit we can determine the coefficient of the linear term and the Zeeman gap for several values of the external magnetic field, as shown in Figs. 10 and 11, respectively. Fig. 10 shows that the coefficient of the linear term in the specific heat is reduced as the external field is applied. The simplest interpretation for this effect is that the Zeeman splitting of the polarized bands causes a decrease in the density of states at the Fermi level (40). This behavior of is quite distinct from that in antiferromagnet heavy fermions (41), as expected from the different roles of in these systems.
The suppression of the magnons by the magnetic field also decreases the low temperature electrical resistivity due to a partial freezing of the electronmagnon scattering. The low temperature electrical resistivity shown in Fig. 12 for T is well described by the expression (42)
(8) 
The gap (units of temperature) extracted from the resistivity data for several values of the applied magnetic field is shown in Fig. 11. The gaps obtained from the transport and thermodynamic data are in satisfactory agreement. The straight line in this plot show the expected value for the Zeeman gap in the simplest (non selfconsistent) spinwave theory (31).
For completeness, we now present magnetoresistance results at ambient pressure for our sample. Resistivity is measured as a function of magnetic field for fixed temperatures below the Curie temperature. For small fields, T and very low temperatures, the magnetoresistance is positive reaches a maximum at and then decreases almost linearly with field for . Magnetoresistance of multiband ferromagnetic metals, like transition metals, has been intensively studied both experimentally and theoretically (43). Raquet et al. (43) have shown that for systems with a light band of conduction electrons and a heavy band of quasiparticles, intraband scattering in the conduction cband can be neglected. Notice that due to the strong hybridization in URuGe (11) the bands have a hybrid character and those referred above are in fact are mostly cband and mostly fband. Considering electronmagnon scattering, which involves intraband and interband spin flip process, Raquet et al. (43) have shown that in the presence of a magnetic field, the magnetoresistance roughly follows a dependence for temperatures above approximately . In Fig. 13 we plot the magnetoresistance defined as as a function of for different fixed temperatures. is the value of the magnetic field for which the magnetoresistance reaches a maximum before starts to decrease. We attribute the positive magnetoresistance at low fields and temperatures to the existence of domain walls that are eventually removed at .
Vii Conclusions
The study of systems close to quantum criticality is an exciting area of research. In the case of itinerant ferromagnets driven to a magnetic instability, there are theoretical and experimental evidences that quantum critical behaviour is avoided and a first order transition occurs before the FQCP is reached (44); (45). In this work we present a thorough investigation of the ferromagnetic heavy fermion system URuGe as it is driven to the paramagnetic state under applied pressure. The results of the transport properties under pressure show no sign of a discontinuous behavior as is reduced. The resistivity curves present no hysteresis effects for any pressure, before and after ferromagnetism is suppressed. Disorder is certainly present in our system, as evidenced by its high residual resistivity. It is possible that the continuous behavior is due to its influence since it substantially modifies the properties of our sample when compared to single crystals (11). However, disorder is not sufficiently strong to give rise to localization effects or Griffith’s singularities. On the contrary, our sample presents many of the properties expected for an itinerant clean system, as the temperature dependence of the resistivity at its FQCP.
URuGe is a unique Uranium compound with negligible anisotropy. This implies that spinwaves, the elementary excitations of a ferromagnetic metal can be easily excited and play a fundamental role in the thermodynamic and transport properties of this system at low temperatures. We have shown that as the FQCP is approached with increasing pressure the spinwave stiffness softens and we obtain its quantum critical behavior. It would be very interesting to measure directly the spinwave stiffness of URuGe by inelastic neutron scattering and compare it to the results we obtained. Specially interesting would be to observe with neutrons the softening of the magnons with increasing pressure.
Although our results are in close agreement with those of Refs. (5) and (10) on the same system, they differ from those obtained in single crystals (11) where a reorientation of the magnetization inside the ferromagnetic phase is observed.
In summary our results on the ferromagnetic URuGe provide strong evidence for the existence of a pressure induced ferropara quantum phase transition in this system that is accompanied by a softening of the elementary excitations of the ordered phase. Its quantum critical behavior shares many features with that expected for a clean, itinerant FQCP.
Acknowledgements.
The authors M.P.N., M.A.C., A.L., A.L., D.C.F., J.L.J., C.E., J.F.O., E.B.S. and M.B.F. would like to thank the Brazilian Agencies CAPES, CNPq and FAPERJ for partial financial support. We thank Prof. Dr. Renato Bastos Guimarães for using the XRay Diffraction Laboratory (LDRX) at the Instituto de Física, Universidade Federal Fluminense (IFUFF).References
 see Strongly correlated electron systems; reports on the progress of the field, Guest Editors, Laura H Greene, Joe Thompson and Jï¿½rg Schmalian, Reports on Progress in Physics, 80, Number 3 (2017); Ye Chen, Zongfa Weng, Smidman Michael, Xin Lu and Huiqiu Yuan, Chinese Phys. B 25 077401 (2016).
 Dai Aoki and Jacques Flouquet, J. Phys. Soc. of Jap. 81 011003 (2012).
 Mucio A. Continentino, Quantum scaling in manybody systems: an approach to quantum phase transitions, Cambridge University Press (2017).
 L. G. Akselrud, J. P. Jarmoljuk, and E. I. Gladyshevskij, Dopov Akad Nauk., 359 (1978).
 S. A. M. Mentink, G. J. Nieuwenhuys, A. A. Menovsky, and J. A. Mydosh, J. Appl. Phys. 69 5484 (1991).
 H. H. Hill, Plutonium 1970 and Other Actinides, edited by W. N. Miner (American Institute of Mining, Metallurgical, and Petroleum Engineers, New York, 1970), p. 2.
 B. Lloret, B. Buffat, B. Chevalier, and J. Etourneau, J. Mag. Mag. Mat. 67 232 (1987).
 E. Colineau, F. Wastin, E. J. Higgins, and J. Rebizant, J. Alloy. Comp. 317, 336 (2001).
 Samir F. Matar, Bernard Chevalier, and Rainer Pöttgen, Solid State Sci. 27 5 (2014).
 Hiroyuki Hidaka, Sosuke Takahashi, Yusei Shimizu, Tatsuya Yanagisawa, and Hiroshi Amitsuka, J. Phys. Soc. Jpn. 80 SA102 (2011).
 Michal Vališka, Martin Diviš, and Vladimír Sechovsky, Phys. Rev. B 95 085142 (2017); Michal Vališka, Milan Klicpera, Petr Doležal, Oscar Fabelo, Anne Stunault, Martin Diviš, Vladimír Sechovský, arXiv:1711.06113 and Phys. Rev. B 97, 125128 (2018).
 Frederic Keffer, in Encyclopedia of Physics, SpringerVerlag, Vol. XVIII/2 pp. 1273 (1966).
 M. Pajda, J. Kudrnovsky, I. Turek,V. Drchal, and P. Bruno, Phys. Rev. B64 174402 (2001).
 J. Mathon, Proc. Roy. Soc. A 306 355 (1968).
 J. Larrea J., M. B. Fontes, A. D. Alvarenga, E. M. BaggioSaitovitch, T. Burghardt, A. Eichler, and M. A. Continentino, Phys. Rev. B 72, 035129 (2005).
 Mucio A. Continentino, Gloria M. Japiassu, Amos Troper, Phys. Rev. 39, 9734 (1989).
 H. M. Rietveld, J. Appl. Cryst. 2, 65 (1969).
 J. RodríguezCarvajal, Physica B 192, 55 (1993); T. Roisnel and J. RodríguezCarvajal, Materials Science Forum 378?381, 118 (2001)
 Institut LaueLangevin, http://www.ill.eu/sites/fullprof/Php/downloads.html.
 George F. Vander Voort, Metallography  Principles and Practice, ASM International, Ohio, 2007.
 D. J. Poutcharovsky and E. Parthe, Acta Cryst. B30, 2692 (1974).
 Ingmar Grenthe, Janusz Drozdzynski, Takeo Fujino, Edgar C. Buck, Thomas E. AlbrechtSchmitt, and Stephen F. Wolf, Uranium in: The Chemistry of the Actinide and Transactinide Elements, volume 1, 3rd edition  Edited by: Lester R. Morss, Norman M. Edelstein and Jean Fuger, Springer, Dordrecht, 2008.
 Nathan R. Gubel. Kenneth H. Eckelmeyer. Kimbberly N. Johnson. Mark J. Jacksone Jonatan S. Morrell, Introduction to Uranium in: Uranium Processing and Properties  Edited by: Jonathan S. Morrell e Mark J. Jackson, Springer, New York, 2013.
 C. P. Susz, J. Muller, K. Yvon, and E. Parthï¿½, J. Less Common Met. 71, 1 (1980).
 Sigurds Arajs, Robert H. Flora, and Elmer E. Anderson, J. Nucl. Mater. 37, 89 (1970).
 L. F. Bates and D. Hughes, Proc. Phys. Soc. B67, 28 (1954).
 C. J. Kriessman Jr and T. R. McGuire, Phys. Rev. 85, 71 (1952).
 C. P. Susz, J. Muller, K. Yvon, and E. Parthï¿½, J. Less Common Met. 71, 1 (1980).
 D. J. Poutcharovsky, K. Yvon, and E. Parthe, J. Less Common Met. 40, 139 (1975).
 see Stephen Blundell in Magnetism in condensed matter, Oxford University Press, p.195196, (2001).
 Frederic Keffer, Spin Waves in: Encyclopedia of Physics: Ferromagnetism. Edited by: H. P. J. Wijn, Chief Editor: S. Flügge, Springer, Berlin, (1966).
 T. M. Palstra, A. A. Menovsky, J. Van den Berg, A. J. Dirkmaat, P. H. Kes, G. J. Nieuwenhuys, and J. A. Mydosh. Phys. Rev. Lett. 55, 2727 (1985).
 W. Schlabitz, J. Baumann, B. Pollit, U. Rauchschwalbe, H. M. Mayer, U. Ahlheim, and C. D. Bredl, Superconductivity and magnetic order in a strongly interacting fermisystem: URuSi In: Ten Years of Superconductivity: 19801990, pages 8995, Springer, 1986.
 S. K. Dhar, R. J. Begum, P. Raj, P. Suryanarayana, L. C. Gupta, and R. Vijayaraghavan, Solid State Commun. 83, 965 (1992).
 T. Mito, M. Hattori, G. Motoyama, Y. Sakai, T. Koyama, K. Ueda, T. Kohara,M. Yokoyama, and H. Amitsuka, J. Phys. Conf. Ser. 391, 012044 (2012).
 B. Lloret, B. Chevalier, P. Gravereau, B. Darriet, and J. Etourneau, J. Phys. Colloq. 49, C8487 (1988).
 R. Troc and V. H. Tran, , J. Mag. Mag. Mat. 73, 389 (1988).
 A. Vernière, P. Lejay, P. Bordet, J. Chenavas, J. P. Brison, P. Haen, and J. X. Boucherle, J. Alloys Compd. 209, 251 (1994).
 D. Belitz, T. R. Kirkpatrick, A. J. Millis and Thomas Vojta, Phys. Rev. B58, 14155 (1998).
 G. R. Stewart, Rev. Mod. Phys. 56, 755 (1984).
 I. Sheikin, Y. Wang, F. Bouquet, P. Lejay and A. Junod, J. Phys.: Condens. Matter 14, L543 (2002).
 N. H. Andersen and H. Smith, Phys. Rev. B 19 (1979), 384. M. B. Fontes, J. C. Trochez, B. Giordanengo, S. L. Budko, D. R. Sanchez, and E. M. BaggioSaitovitch and M. A. Continentino, Phys. Rev. B60, 6781 (1999).
 B. Raquet, M. Viret, E. Sondergard, O. Cespedes, and R. Mamy, Phys. Rev. B66, 024433 (2002) and references therein.
 M. Brando, D. Belitz, F. M. Grosche, and T. R. Kirkpatrick, Rev. Mod. Phys. 88, 25006 (2016).
 Alexander Steppke, Robert Küchler, Stefan Lausberg, Edit Lengyel, Lucia Steinke, Robert Borth, Thomas Lühmann, Cornelius Krellner, Michael Nicklas, Christoph Geibel, Frank Steglich, Manuel Brando, Science 339, 933 (2013).